Atmospheric Corrosion of Austenitic Stainless Steels
Steven Richard Street
A thesis submitted to the University of Birmingham for the
degree of DOCTOR OF PHILOSOPHY
School of Metallurgy and Materials
College of Engineering and Physical Sciences
University of Birmingham
University of Birmingham Research Archivee-theses repository
This unpublished thesis/dissertation is copyright of the author and/or third parties. The intellectual property rights of the author or third parties in respect of this work are as defined by The Copyright Designs and Patents Act 1988 or as modified by any successor legislation.
Any use made of information contained in this thesis/dissertation must be in accordance with that legislation and must be properly acknowledged. Further distribution or reproduction in any format is prohibited without the permission of the copyright holder.
Atmospheric corrosion was investigated using electrochemical and droplet studies. The effects of changes in bulk solution concentration and local pit chemistry on pit propagation and repassivation of 304L and 316L stainless steels were investigated using in situ synchrotron X-radiation and electrochemical techniques.
Radiography and zig-zag electrochemical sweeps showed that in dilute chloride solutions, partial passivation was observed to initiate locally and propagate across the corroding surface. This caused repassivation gradually rather than as a uniform event. In concentrated chloride solutions, repassivation did not show a sudden drop in current but rather a gradual decrease as potential swept down. Pitting behaviour was also affected by solution concentration. Dilute solutions showed metastable pitting followed by a sharp breakdown (pitting) potential. Concentrated solutions however showed no metastability and a gradual increase in current when pitting. To determine the cause of current oscillations in 304L artificial pits in NaCl:NaNO3 solutions near the repassivation potential, the salt layers were scanned in situ using
XRD. The salt layer was confirmed to be FeCl2.4H2O and no nitrate salt was found. A mechanism was suggested to explain the current oscillations in terms of partial passivation being undercut by the advancing corrosion front.
The morphology of pits caused by atmospheric corrosion of 304L plate under droplets of MgCl2 was investigated. Changes in pit morphology were linked to relative humidity and droplet thickness. Initial pit morphology showed a shallow dish region, which is suggested to be caused by elevated passive current dissolution under high concentrations. Position of pits under the droplet was linked to initial
solution concentration. Distinctions between Aerosol and “Splash zone” salt depositions were investigated.
A great many people helped to guide me through this body of work and I am sincerely thankful to each of them.
Both my supervisors, Prof Alison Davenport and Prof Trevor Rayment, have shown inexhaustible patience with the meandering path that my research has taken. Many thanks to them and also to all my colleagues in the corrosion research group, who are too numerous to name but have helped me immensely.
I gratefully acknowledge all the assistance that I have received from Diamond Light Source Ltd., particularly Dr Fred Mosselmans and Dr Mahrez Amri of I18, Dr Paul Quinn of I14, Dr Christoph Rau and Dr Joan Vila-Comamala of I13, and Dr Mark Basham of the Software Development Team.
Finally, I would like to thank my family for their continued support, love, and encouragement.
Dedicated to my wife and my daughter.
“When I was a child, I spake as a child, I understood as a child, I thought as a child: but when I became a man, I put away childish things.”
1. Introduction ... 1
2. Literature review ... 4
2.1. Austenitic stainless steel ... 4
2.2. Pitting Corrosion of stainless steels ... 5
2.2.1. Introduction ... 5
2.2.2. Initiation of pitting ... 6
2.2.3. Propagation of pitting... 8
2.2.4. Metastable pits ... 10
2.3. One dimensional pitting ... 10
2.3.1. Geometry ... 10
22.214.171.124. Measuring Pit Depth ... 15
2.3.2. Salt layers ... 15
2.3.3. Current Voltage Characteristic ... 17
2.3.4. Tafel slope ... 18
2.4. Passivation ... 19
2.4.1. Role of nitrate on steels ... 22
2.4.2. Role of molybdenum in stainless steel ... 24
2.5. Atmospheric Pitting Corrosion ... 25
2.5.1. Salt deposition ... 26
2.5.2. Deliquescence ... 26
2.5.3. Evans Droplet Model ... 27
2.5.4. Secondary spreading of droplets ... 29
2.5.5. Laboratory simulation ... 30
2.5.6. Morphology of pits... 31
2.6. Synchrotron Sources ... 33
2.6.1. What is a synchrotron? ... 33
2.6.2. X-ray Diffraction on corrosion systems ... 34
2.6.3. Radiography ... 35
2.6.4. Effect of X-radiation on electrochemical data ... 36
3. Experimental procedures... 37
3.1.1 SEM and EDS characterisation of alloys ... 38
3.2. Salt solutions ... 40
3.3. Synchrotron Experiments ... 40
3.3.1. Synchrotron sample preparation ... 40
3.3.2. Synchrotron XRD experiments ... 41
3.3.3. Synchrotron Radiography experiments ... 43
3.4. Atmospheric corrosion droplet experiments ... 44
3.4.1. Sample preparation ... 44
3.4.2. Atmospheric Experiments ... 44
3.4.3. Time-lapse experiments ... 46
3.4.4. Droplet Ag wire experiments ... 46
3.5. One-dimensional pitting experiments ... 47
3.5.1. Sample preparation ... 47
3.5.2. Electrochemical measurements ... 48
3.5.3. Zig-zag pitting ... 48
3.6. Wire experiments ... 49
3.7. Full immersion plate experiment ... 50
4. Effect of nitrate on the salt layers in artificial pitting corrosion of 304L stainless steel 51 4.1. Introduction ... 51 4.2. Results ... 52 4.2.1. Electrochemistry ... 52 4.2.2. SEM Results ... 55 4.2.3. Diffraction results ... 56 4.2.4. Radiography results... 59
4.2.5. Corrosion front roughness results ... 62
4.3. Discussion ... 64
4.4. Conclusions ... 70
5. Atmospheric corrosion of 304L stainless steel under droplets of MgCl2... 72
5.1. Introduction ... 72
5.2. Results ... 73
5.2.1. Time-lapse growth ... 77
5.2.2. Pit Morphologies ... 79
5.2.4. Statistical analysis of the effect of RH and CDD on Pit Location ... 84
5.2.5. Measuring inner and outer droplet areas ... 84
5.2.6. Statistical Analysis ... 86
5.2.7. Effect of changes in Relative Humidity (RH) on pitting position ... 87
5.2.8. Effect of solution concentration ... 90
5.2.9. Ag wire electrochemistry ... 92
5.3. Discussion ... 94
5.3.1. Pit Morphology ... 94
5.3.2. Pit Position ... 97
5.4. Conclusions ... 102
6. Electrochemical studies on 304L and 316L in highly concentrated MgCl2 solutions using 1D artificial pits and wire electrodes ... 105
6.1. Introduction ... 105
6.2. Results ... 106
6.2.1. One-Dimensional pitting ... 106
6.2.2. Zig-zag sweeps ... 108
6.2.3. Electrochemical Impedance spectroscopy (EIS) ... 114
6.2.4. Effect of pit depth growth ... 114
6.2.5. Wire Electrochemistry ... 121
6.3. Discussion ... 130
6.3.1. Pitting ... 130
6.3.2. Repassivation ... 133
6.3.3. Passive Current Density ... 134
6.3.4. Application of EIS to one-dimensional pitting ... 136
6.3.5. Application to atmospheric corrosion ... 137
6.4. Conclusions ... 139
7. General Discussions and Future Work ... 141
7.1. Synchrotron studies ... 141
7.1.1. Identification of nitrate-rich salt with XRD ... 141
7.1.2. Use of radiography to isolate partial passivation mechanism ... 141
7.2. Electrochemistry of Atmospheric Corrosion ... 141
7.2.1. Pitting Behaviour in ‘atmospheric’ conditions ... 142
7.3. Role of Molybdenum in atmospheric corrosion... 144
7.4. Analysis of corrosion under droplets ... 145
7.5. Future Work ... 147
7.5.1. More accurate EIS data to isolate critical values using TRFT-EIS ... 147
7.5.2. In Situ investigation of partial passivation and repassivation ... 148
7.5.3. Nitrate Reduction Mechanisms ... 148
7.5.4. Role of Molybdenum in concentrated solutions. ... 149
8. Conclusions ... 150
v LIST OF SYMBOLS AND DEFINITIONS
A surface area
ba Tafel slope
D average diffusivity
DH Deliquescence Humidity
Eapp Applied potential
Ecorr Corrosion Potential
Epass Primary passivation potential
Epit Pitting potential
Erp Repassivation potential
F Faraday constant
H0 Null Hypothesis
i current density
ia anodic current density
icorr open circuit corrosion current density
ilim diffusion-limited current density
Ilim diffusion-limited current
Int transmission beam intensity
Int0 original beam intensity
Mw average molecular weight of an alloy
n average valency of an alloy
ni integer for Bragg equation
Q total charge passed
R Universal gas constatn
RH Relative Humidity
RSD Surface Roughness
Rj Roughness and point j
Rm Mean roughness
wt% weight per cent of alloy
x pit depth
xt absorption thickness
ΔC difference in metal ion concentration between the corrosion interface and the bulk solution
μ absorption coefficient
ρ average alloy density
σH0 Binomial standard deviation of the null hypothesis
φs IR-drop across solution
φsf IR drop across salt film χ2 Chi-squared
Austenitic stainless steels are currently used in the United Kingdom to build containers to store Intermediate Level Nuclear Waste (ILW), with 304L and 316L alloys being the primary choices. The eventual plan for this waste is to place it underground in a geological disposal facility permanently . However, this facility has not yet been built and it may be one hundred years before it will be ready to accept ILW. In the meantime, ILW containers are kept in warehouses that are vulnerable to salty aerosol deposits . These aerosol deposits come from a variety of sources, such as crashing waves in the sea , and commonly have salt species in them. There are other species amongst the salts, such as nitrates which are thought to originate from farming contamination. Nitrates are known to cause surges in
electrochemical dissolution, yet the mechanism explaining this has not been confirmed. There is a risk that over the next century, atmospheric corrosion may occur on these ILW containers and provide initiation sites for stress corrosion cracking to occur, causing the containers to fail when being moved from interim storage to their final destination.
The salts that are deposited on the surface of these containers are hygroscopic, i.e. draw in moisture from the surrounding atmosphere . As humidity fluctuates throughout the year it is possible for these salts to draw in enough moisture to become highly concentrated saline solutions. This leads the stainless steel to be vulnerable to localised corrosion. The humidity at which a salt begins to draw in moisture is known as its “deliquescence” humidity, which is a thermodynamic property for each salt. MgCl2 is of particular relevance in atmospheric corrosion due
to its presence in sea water and aerosol depositions, and its relatively low deliquescence RH that is commonly quoted as 33% at 30 °C .
Recent developments in synchrotron techniques have allowed the observation of pitting behaviour in situ using a range of techniques X-ray diffraction [6, 7] and radiography[8-10]. The high flux and high resolution of synchrotron techniques allow time-resolved results to be collected and correlated with electrochemical data. Atmospheric corrosion occurs in highly concentrated solutions, although the vast majority of electrochemical corrosion investigations have occurred in dilute
solutions. There has been some evidence that the behaviour of corrosion changes in higher concentrations [11, 12], so further investigation in conditions comparable to those in atmospheric corrosion is warranted.
As pit morphologies are complicated, one-dimensional artificial pitting electrodes have been used to simplify analysis of results . The regular geometry of these pits allows realistic values of current density and threshold potentials to be collected, such as the transition between diffusion-limited dissolution and active dissolution, and active dissolution and repassivation.
The principal aims of this body of research are to investigate the localised corrosion of 304L and 316L in terms of interfacial kinetics and repassivation. The influence of nitrate on the mechanism of repassivation of 304L is here investigated using
synchrotron radiation to analyse the corroding salt layer during dissolution and when a near repassivation in addition to electrochemical analysis . Repassivation of 304L and 316L in MgCl2 solutions are conducted in highly concentrated solutions to
give insight on repassivation behaviour in atmospheric corrosion conditions, as repassivation is most commonly described in terms of dilute solutions [15, 16]. The influence of initial solution concentration of droplets of MgCl2 on both the morphology and the position of pitting of 304L is also investigated. This will allow analysis of principal mechanisms of propagation in pits found in service that do not often conform to morphologies predicted by electrochemical models of corrosion [13, 17].
2.1.Austenitic stainless steel
Stainless steels are Cr-rich steels that are highly resistant to general corrosion due to the growth of very stable chromium oxide film on the metal surface. A steel is stainless if it is able to regenerate this chromium oxide layer film after damage, usually requiring at least 11 wt% Cr in solid solution to allow this .
There are generally considered to be four categories of stainless steels: ferritic, martensitic, austenitic and duplex . Although steel maintains a face centre cubic (FCC) crystal structure at elevated temperatures, this normally reverts to body centre cubic (BCC) as the alloy cools. The addition of FCC stabilisers, such as Ni, allows FCC structure to be maintained at low temperatures. 300 series alloys have 18 wt% Cr is added to maintain a durable passive layer and promote corrosion resistance. As Cr acts as a ferrite stabiliser, promoting BCC crystal structure at room temperature, 8-10 wt% Ni is also added to maintain the FCC structure.
The most common austenitic grades are 304 and 316 stainless steels, each with approximately 18 wt% Cr and 10 wt% Ni. 316 has an additional 2-3 wt% Mo which has been observed to enhance its ability to prevent pitting corrosion . Low carbon grades of these alloys are denoted with ‘L’ as a suffix: 304L and 316L. These are desirable as they prevent the formation of carbides at grain boundaries that may locally reduce Cr content in solid solution.
2.2.Pitting Corrosion of stainless steels
Stainless steels are generally considered to have excellent resistance against general corrosion because of the very stable chromium oxide film that reforms after it is damaged by any scratches in normal use. However, they are susceptible to localised corrosion caused by defects and surface-breaking inclusions in the material
microstructure. These inclusions form from alloying elements and impurities introduced during the iron- and steel-making phases of production.
Figure 2-1 Schematic diagram of the key processes involved in pitting of metal in NaCl solution. Anodic reaction is the dissolution of metal and cathodic reaction is the oxygen reduction reaction.[20, 21].
Pitting is an autocatalytic process (Figure 2-1) where the propagation of pitting creates an environment more susceptible to corrosion. This is enabled by the occluded morphologies generated during the pitting process.
6 2.2.2. Initiation of pitting
126.96.36.199. Role of Sulphur during solidification
The initiation of pitting in stainless steels has been most widely attributed to the presence of surface-breaking inclusions on the metal surface . Although other mechanisms have been suggested, these generally focus on the structure of the oxide film and are independent of underlying inclusions [23-26] and are most useful in explaining very clean systems such as deposited thin films. Bulk alloys, such as austenitic stainless steels, are typically discussed in terms on initiation at an inclusion .
Sulphide inclusions are considered the most significant type of inclusion when considering pitting initiation of stainless steels . Sulphur (S) is introduced into the alloy as an impurity from ore and coke supplies  and great pains are taken to remove sulphur from the melt, particularly in the iron-making stage. Alloying additions are used to remove S by reacting it to float off as a buoyant slag. Most commonly lime (CaO) is added but Mg, Na and rare earths are also used.
Not all S can be economically removed in this way and to further mitigate its effect on the alloy elements, such as Mn, are added to the alloy . Mn forms MnS at 1650 °C, 80 degrees above the solidus temperature of the bulk, allowing the overwhelming majority of S in the alloy to be reacted with Mn without preference for grain boundary positions. MnS is also quite ductile, so does not form voids or sharp stress concentrators as it is rolled or formed. Although some stainless steels contain relatively high amounts of S (~0.3 wt%) to improve machinability, e.g.
SS303, most austenitic stainless steel alloys aim to have S content below 0.08 wt% and often below 0.03 wt% .
188.8.131.52. Role of MnS inclusions
Localised corrosion in stainless steels was suspected to be influenced by S inclusions long before initiation mechanisms were established [30, 31]. Eklund  developed a Pourbaix diagram for MnS and showed sulphides are not thermodynamically stable at the potentials experienced by passive steels, resulting in the lowering of pH locally. Eklund also suggested an initiation mechanism where “virgin” steel under a newly dissolved sulphide is able to be attacked.
Wranglen  observed pitting initiating under sulphide inclusions in steel,
commenting that the inclusions were less noble than the surrounding matrix and their dissolution resulted in pit solution with higher salt concentration, lower oxygen concentration and lower pH. Wranglen rejected Eklund’s idea that the MnS is an anode, which would “shower” the surrounding matrix with S. Instead, Wranglen suggests S2- and HS- strongly adsorb to the surface of metal, reducing activation overpotential.
Castle and Ke  suggest a sulphite intermediary existed that lowers local pH to help stabilise pitting. The importance of the intermediary thiosulphate species has been observed to lower pH and stabilise pitting during sulphide dissolution . A suggested mechanism for this is :
2𝑀𝑛𝑆 + 3𝐻2𝑂 → 2𝑀𝑛2++ 𝑆
2𝑂32−+ 6𝐻++ 8𝑒− Equation 2-1
𝑀𝑛𝑆 + 2𝐻+ → 𝑀𝑛2++ 𝑆 + 𝐻
It has been suggested that preferential dissolution of Cr at the S inclusion interface is the key feature that promotes the stability of pitting around sulphide inclusions  but this has not been broadly accepted [37, 38]. However, preferential attack around the edge of sulphide inclusions has been observed using scanning auger microscopy  and optical microscopy [40, 41].
Williams et al. have shown a FeS region around sulphide inclusions up to 100 nm thick using secondary ion mass spectroscopy. They hypothesised that this will lead to the formation of a polysulphide skin around the inclusion that will trigger its dissolution.
2.2.3. Propagation of pitting
The growth of pits after initiation depends on the ability of the solution around the corroding surface to maintain an aggressive concentration and resist repassivation, i.e. the maintenance of a critical concentration . In terms of electrochemical potential, a pit can be considered to propagate as long as the interfacial potential is above the repassivation potential, Erp. However, Erp varies in definition between authors and applications, which will be discussed later.
Hoar  first suggested that an autocatalytic mechanism could be responsible for the sustainability of pitting propagation, with the chemistry inside the pit being different than that of the bulk. In neutral solutions, evidence of a significant drop in pH was observed in inside pits [45, 46] and this was achieved by hydrolysis caused by metal ion (M) release:
𝑀 → 𝑀𝑛++ 𝑛𝑒− Equation 2-3
2𝑂 ⇌ 𝑀𝑂𝐻(𝑛−1)++ 𝐻+ Equation 2-4
This reduction in pH destabilises any passive film growth, maintaining actively corroding surfaces. The release of large volumes of cations into the pit causes a charge imbalance, which is corrected by the electromigration of anions from the bulk solution into the pit . Cl- is a particularly aggressive anion as it acts like a strong acid when in solution, i.e. it remains fully dissociated from free H+ions. This allows a high concentration of H+ ions to remain in the pit, further lowering pH. Though there is generally believed to be very little convection inside pits , the constant diffusion of ions away from the corrosion interface requires a restricted diffusion pathway to ensure the number of ions being generated is greater than the number of ions exiting the pit. As such, an occluded geometry is typically required for
corrosion to continue, resulting in a “pit” morphology (Figure 2-1).
The occluded pit geometry creates an ion concentration gradient inside the pit with a saturated solution at the corrosion interface. Continued corrosion supersaturates this solution, causing the precipitation of a salt layer that settles at the bottom of the pit .
The main cathodic reaction in aqueous corrosion of steels is generally acknowledged to be the Oxygen Reduction Reaction (ORR):
The high mobility of electrons through metal allows cathodic and anode reactions to occur at different places on the metal surface, as long as there is a sufficient ion pathway through the solution to allow charge balance. The generation of hydroxyl ions at the cathode increases pH locally, provide cathodic protection against attack in these regions.
2.2.4. Metastable pits
Not all initiation events stabilise into propagation of pits. Those that fail to grow are labelled “metastable”, though this is only known after failure to pit as they share the same mechanism of initiation as successful pits . In these cases, although the dissolution of an inclusion occurs, the pitting site is not occluded enough to maintain an aggressive chemistry, so rapidly repassivates . Solution chemistry can affect metastable pitting. In dilute solutions, Pistorius and Burstein observed reducing NaCl solution concentration from 1 M to 0.01 M reduced the occurrence of
metastable pitting on 304 stainless steel. They also observed that reducing pH from 9 to 7 increased metastable pitting. Solution concentration also affects metastable pitting, with fewer metastable pits present in highly concentrated solutions of MgCl2 on 304L .
2.3.One dimensional pitting
The complicated geometry of pits allows different regions inside the pit to experience different corrosion behaviours, as explained above. This makes the interpretation of electrochemical data challenging as the current drawn from pits was averaged over the entire pit interface, and it is difficult to isolate physical geometries
of a growing pit in a wire or plate surface. One dimensional pits, or artificial pits, were developed as an experimental model to better understand the electrochemistry recorded during pitting experiments. Pickering and Frankenthal [50, 51] first developed the “unidirectional” model of pitting for metals in acidic solutions,
considering diffusion and migration of ions but not convection as it was viewed to be negligible. Galvele  further simplified Pickering’s model by accounting only for metal ion diffusion and expanding its utility to any pH bulk solution.
One-dimensional pitting occurs when artificial pits are of a sufficient depth that diffusion along the pit is uniform. As seen in Figure 2-2a, corrosion begins with a pit depth of zero, allowing hemispherical diffusion through the bulk solution. As the pit grows, diffusion from the corrosion front is increasingly restricted by the occluded geometry of the pit, allowing solution at the interface to supersaturate and precipitate a salt layer (Figure 2-2b). There is still significant hemispherical diffusion at the pit
mouth, however. As the pit continues to grow, hemispherical diffusion of metal ions from the pit mouth will become negligible, meaning in uniform diffusion in the pit (Figure 2-2c). This results in one-dimensional pitting, and electrochemistry can be interpreted as uniform across the surface of the anode.
Isaacs  showed the development of resistive layers in one dimensional crevices, suggesting that these were most likely metal chloride salts due to their solubility and diffusion effects, as highly concentrated bulk solutions reduced current significantly.
Figure 2-2 Schematic model of one-dimensional pitting experiment. (a) Metal wire embedded in non-corroding polymer initially corrodes with hemispherical diffusion at the pit mouth. (b) Pit with salt layer and some hemispherical diffusion at pit mouth. (c) One-dimensional pit where hemispherical diffusion at pit mouth is negligible.
Beck , using titanium cells, also concluded that the drop in potential in the steady state condition was due to the formation of a porous salt layer. Tester and Isaacs  went on to develop one-dimensional pitting model assuming a quasi-steady state condition where corrosion rate is controlled by diffusion with a concentration gradient being the driving force. They observed this behaviour in a range of metals, proposing a chloride salt being responsible for the independence of current to applied voltage in each case. The quasi-steady state period is observed after an initial “transient” period, where local pit chemistry is being established at shallow depths (Figure 2-3).
Figure 2-3 Schematic diagram from Tester and Isaacs  showing the initial growth of a one-dimensional artificial pit under constant potential. The “transient” region where the pit grows until a salt layer forms at time τ, after which is a region of quasi-steady state attack.
By simplifying the model to account only for mass transport by diffusion, not convection or migration, Tester and Isaacs  showed a relationship can be made between current and pit depth. For a wire with a fixed cross-section, the flux of metal ions away from the corrosion interface can be expressed as:
𝑁 =𝐴𝑛𝐹𝐼 Equation 2-6
Where N is the cation mass flux from the interface, I is the current, n is the average number of electrons liberated per cation, F is the Faraday constant, and A is the wire cross-sectional area. The loss of cations at the metal interface will be driven by two processes, namely a concentration gradient and a potential gradient. This can be expressed using the Nernst-Einstein equation
𝐼 𝐴𝑛𝐹= 𝐷 [ 𝛿𝐶 𝑑𝑥+ 𝐶̅ 𝑛𝐹 𝑅𝑇𝐷 𝛿𝜙 𝛿𝑥] Equation 2-7
Where D is the ionic diffusion coefficient, δC is change in metal cation
concentration, δx is change in pit depth, R is the universal gas constant, T is the temperature of the system in K, C̄ is the average metal ion concentration in the pit,
δΦ is the change in potential. The potential gradient in this system has been observed to have no significant impact in mass transport in one-dimensional pitting under a salt layer, so the equation can be reduced to only consider mass transport via diffusion:
𝐼 𝐴𝑛𝐹= 𝐷
𝛿𝑥 Equation 2-8
Simplifying and integrating both sides gives:
∫𝑥𝑥𝑚𝑎𝑥𝐴𝐼 𝑚𝑖𝑛 𝛿𝑥 = ∫ 𝑛𝐹𝐷 𝐶𝑠𝑎𝑡 𝐶𝑏𝑢𝑙𝑘 𝛿𝐶 Equation 2-9 𝐼 𝐴[𝑥 − 0]= 𝑛𝐹𝐷[𝐶𝑠𝑎𝑡− 𝐶𝑏𝑢𝑙𝑘] Equation 2-10
Where xmax is the pit depth, xmin is the top of the pit (i.e. 0), Csat is the saturation concentration of metal ions at the corrosion interface and Cbulk is the concentration of metal ions in the bulk. This can be rearranged to give the diffusion limited current density of the pit :
𝑖𝑙𝑖𝑚 =𝑛𝐹𝐷∆ 𝐶𝑥 Equation 2-11
Where i is the limiting current density in the pit and ΔC is Csat – Cbulk. As n, F, D, and ΔC are broadly constant, another relationship can be established:
𝑖𝑙𝑖𝑚𝑥=𝑛𝐹𝐷∆ 𝐶 Equation 2-12
ilimx is known as the pit stability product  and is constant if one dimensional
diffusion gradient at the mouth of the pit is negligible and pitting can be treated as one-dimensional . Woldemedhin et al.  used stainless steels in FeCl3 and LiCl with concentrations up to 8.58 M [Cl] to observe a decrease in pit stability product (ix) with increasing solution concentration. Artificial pits have also been extended into two dimensions to see growth under diffusion and ohmic control [8, 55]
184.108.40.206. Measuring Pit Depth
Radiography analysis of 304L corrosion in chloride solution  has shown that metal lost during 1D pitting experiments is via electrochemical dissolution and very little is lost by flaking, spalling or undercutting. As such, it can be assumed that current can be used to calculate material loss and pit depth during dissolution. The total charge passed during dissolution, Q, is the integration of the current over time. Pit depth can be calculated using Faraday’s Second law :
𝐴𝑛𝐹𝜌 Equation 2-13
where x is pit depth and A is surface area of pit, Mw is average molecular weight of alloy, n is average valence of alloy, F is Faraday Constant and ρ is average alloy density. This method of measuring material loss has shown high levels of
repeatability for austenitic stainless steels when compared to optical measurements [57, 58].
2.3.2. Salt layers
Salt layers are formed when solutions inside the pit have become supersaturated with ions during high anodic dissolution. Supersaturation is a necessary step to precipitate
a salt layer  with current density required to nucleate a salt layer ranging from 1.8 times to 5 times the diffusion limited current density [15, 60, 61]
Salt layers are in a dynamic equilibrium with the pit solution and are continually dissolving and reforming while corrosion continues . Isaacs  showed that corroded 304L stainless steel one-dimensional pits in chloride solutions and have salt layers that are highly resistive. The salt layer at the bottom of a pit was originally believed to be non-porous, but this idea was refined to include a hydrated layer that allowed water to pass through it . Danielson then investigated the response of the salt layer to incremental steps in applied current, coming to the conclusion that it should be considered a porous layer . Landolt et al.[64-66] suggested a “duplex” structure of the salt layer, with a compact anhydrous region at the corrosion interface and a loosely packed region closer to the bulk solution. This model was developed using results from Fe and Ni alloys. This duplex model has been used to calculate porosity of outer regions of salt layers in Fe systems in chloride solutions . The structure of salt layers has been investigated in situ using a range of methods. Sridhar and Dunn  used Raman to identify the salt layer at the bottom of a Ni pit to be NiCl2.6H2O. X-ray diffraction has recently been used on one-dimensional pits of austenitic stainless steels and Fe to show FeCl2.4H2O salt layers . Diffraction patterns were also able to show anisotropy, indicating a texture under some corrosion conditions [6, 69]. At the corrosion interface, FeCl2.2H2O has been observed in 304L and 316L stainless steels  indicating a reduction in access to water.
17 2.3.3. Current Voltage Characteristic
Figure 2-4 shows a typical current-voltage characteristic diagram for a one-dimensional pit that has been pre-grown, i.e. is of a sufficient pit depth to make hemispherical diffusion at the pit mouth negligible . Starting at point A, the potential is increased at a constant rate. The region between A and C is under ohmic control, i.e. current response is proportional to the potential applied to the system. The solution at the pit interface continues to get more saturated as corrosion continues and will eventually get supersaturated. At point C the supersaturated solution reaches capacity and a salt layer precipitates out. This salt layer is resistive so current drops to nearly zero, as seen at point D. The precipitation of a large
amount of salt from the supersaturation solution leaves the system out of equilibrium. The salt layer then thins as the system approaches equilibrium again. By point E, the system is at equilibrium and the limiting current, Ilim, has been reached. As the potential gradually increase, no change in current is observed. The system is under “diffusion control” here, and any increase in applied current will be absorbed by a thickening of the salt layer.
When the potential sweep is reversed from point E and lowered gradually, current remains constant at Ilim. While the potential decreases, the salt layer thins. At point F, applied potential has become so low that the salt layer can no longer be maintained and it dissolves fully. This point is known as the Transition Potential, ET, and marks the transition between diffusion controlled and activation controlled dissolution. As potential sweeps down to point G, the current decreases until passivation.
Figure 2-4 Current-Voltage characteristic of a one-dimensional artificial pit of a pre-grown pit. Applied potential increases .
2.3.4. Tafel slope
The Tafel slope is a measurement that relates anodic dissolution kinetics to the overpotential (i.e. the difference between the applied potential and the reversible potential of a reaction). In one-dimensional pitting, the Tafel slope is measured when corrosion is under activation control. Laycock and Newman , using Beck and Alkire’s  and Galvele’s  observations, proposed a model using voltage balance to calculate IR drop across the corroding interface:
𝐸𝑎𝑝𝑝 = 𝐸𝑐𝑜𝑟 � + 𝑏𝑎𝑙𝑜𝑔 ( 𝑖𝑎
𝑖𝑐𝑜𝑟𝑟) + 𝜙𝑠+ 𝜙𝑠𝑓 Equation 2-14
Where Eapp is applied potential, Ecorr is corrosion potential, ba is the anodic Tafel slope, ia is the anodic current density, icorr is the open circuit corrosion current density, φs is IR-drop across solution and φsf is the IR-drop across the salt film. This relationship can be used for both salt covered and salt free corrosion interfaces.
Anodic dissolution kinetics in near-saturation conditions at the corrosion interface have been investigated by Newman and Isaacs , using IR-corrected potential to find the Tafel slope. In austenitic stainless steel (19-10 alloy) the Tafel slope was measured to be 60 mV/decade when above -300 mV (vs SCE) and 75 mV/decade when below -300 mV. This led to the suggestion that there may be a change in speciation at lower potentials. Other authors have found a range of Tafel values on stainless steels. Gaudet et al.  measured a value of 54 mV/decade on 304L stainless steel in supersaturated solution. Enerhaug et al. measured 57 mV/decade on martensitic steel . However, some results have shown Tafel values of over 100 mV/decade. Steinsmo and Isaacs  measured a Tafel slope of 108 mV/decade on Ferritic stainless steel in supersaturated solutions. Laycock and Newman  measured 110 mV/decade in 302 stainless steel in 1 M NaCl, but this cell may not have been fully IR-corrected as the IR-drop inside the pit was not calculated, only that of the bulk solution .
Fe is generally considered a ‘reactive metal’, i.e. a metal that spontaneously reacts with oxygen or water in ordinary use . James Keir  showed that the treatment of iron with nitric acid prevented the precipitation of silver from silver nitrate while maintaining a shiny surface. Reactive metals, such as Fe, do not however revert to their ore-like state immediately after casting because of kinetic barriers that are formed during the process of ‘passivation’.
Fontana  defines passivity as “the loss of chemical reactivity under certain environmental conditions”. Passivity in stainless steels can be observed
electrochemically using a current-voltage characteristic plot (Figure 2-5). As the potential is increased from Ecorr, the dissolution rate increases with an ohmic relationship in the ‘active’ region. Active dissolution under potentials above Ecorr occurs without the presence of a salt film on the corroding surface. Once the Primary Passivation Potential, Epass, is reached, current drops dramatically and further
increase in potential after this point does not correspond to an increase in current. This indicates the formation of a surface film that impedes the dissolution of underlying metal. This is largely attributed to the formation of adsorbed hydrated complexes of metals, which then react with water to allow the formation of a stable layer . Increasing potential further into the ‘transpassive’ region drives the
Figure 2-5 Schematic diagram of anodic dissolution of a Cr-rich Fe alloy. Epass= primary passivation potential, Ecorr=corrosion potential, icrit= critical current density, ipass=passive current density.
system to return to an approximately linear response in current. This accelerated dissolution is not necessarily due to pitting but most commonly due to the start of new anodic processes .
Repassivation of pits is crucial in determining the sustainability of pitting. Pourbaix et al.  conducted a series of experiments on stainless steels in chloride solutions
and described it as the potential below which pitting current drops below passive current level. Wilde and Williams  showed that in 304 stainless steel neither passivation nor repassivation potentials are material properties and are in fact dependent on environmental and solution conditions.
The concept of repassivation potential was first described by Pourbaix et al. as a “protection tension” , which was developed by Starr et al. suggesting protection may result from a repassivation of an active surface. Here it was determined to be the potential where, once potential was increased, no significant current increase was observed. This has been adopted as a standard definition of Erp . Other definitions include the start of cathodic current on the pitting surface  or then the current density drops below an arbitrary threshold current density value [81, 82], which is in fact the definition used in Pourbaix diagrams. When potentiodynamic sweeps are used on bulk electrodes, such as wires, some authors define Erp as the point where the reverse sweep crosses the forward sweep,
completing a “hysteresis loop” . The selection of the criteria for the definition of Erp does not necessarily depend on the transition between two competing regimes of
ohmic response to variation in potential is observed until very low current densities .
Solution concentration has a strong effect on repassivation. Yashiro and Tanno  observed that pitting potential, Ep, and repassivation potential, Erp, decreased linearly with logarithmic increase of NaCl concentration between the range of 0.1 and 3 M in 304L stainless steels. Anderko et al.  verified these results by showing Erp decreased linearly with logarithmic increase of chloride activity up to saturation, though with two distinct trends: a much steeper decrease occurred at lower concentrations than at higher concentrations. Okada  developed a model for repassivation of a pit, where local islands of oxide appear as the potential approached Erp. This oxidation reduces local dissolution, propagating the passive layer as
2.4.1. Role of nitrate on steels
Nitrate is known to prevent corrosion on stainless steels by acting as a strong
passivating agent [87, 88]. John Keir described the range of effects of nitrate on steel over 200 years ago, showing that concentrated nitric acid protects steels from
corrosion but dilute acid exacerbates corrosion significantly [76, 89]. Lillard et al. have also shown that passive layers form more quickly and are thinner in higher nitrate concentrations .
When trace nitrate is added to chloride solutions a passivation potential is observed, Epass, above which a corroding surface will passivate [91-94]. A correlation has been
observed between Epass and chloride:nitrate ratio, with increasing nitrate concentration resulting in reduced Epass [92, 95].
Just before Epass, current oscillations and fluctuations have been observed [14, 96, 97]. This has been seen as a clue as to the mechanism that operates in passivating stainless steel surfaces in chloride/nitrate solutions. Several theories have been proposed to account for these oscillations:
1. A nitrate-rich salt layer may be formed, with oscillations resulting from competing salt species being formed . This salt may occur as a molten salt, as seen in corrosion of iron in concentrated NaNO3 solutions under high potentials [98, 99], and as such the reduced porosity my increase the
resistivity of these salts.
2. A competitive adsorption, as proposed by Leckie and Uhlig , between chloride and nitrate ions on the corroding surface. This model accounts for the induction time required as competitive adsorption is kinetically limited. This theory is informed by a literature proposing models of protons being cyclically repelled and attracted to the corrosion surface , altering local pH and generating oscillations in current.
3. Nitrate reduction models that consume H+ ions at the corroding surface and raise pH causing passivation [14, 96, 97]. Evans suggested that the reduction of nitric acid was auto-catalytic  on steel and showed this by
augmenting nitrite content in nitrate solutions. Increasing nitrite
concentration in these nitrate solutions increased cathodic current density, indicating reduction reactions. Autocatalytic reaction sequences were later suggested  that involved the reduction of nitrate via adsorption to the pit surface (Vetter’s mechanism)  and in solution near the corroding surface (Schmid’s mechanism) . The electroreduction of NH+ to NO3- as a
possible route that has been put forward  but no direct evidence for this has been observed in the corrosion of austenitic stainless steels . Carbon steel in nitrate/nitrite solutions is known to evolve bubbles which have been hypothesised to be N2, suggesting reduction processes . Temperature has also been observed to influence oscillation behaviour, with higher temperatures reducing their occurrence .
2.4.2. Role of molybdenum in stainless steel
Empirical studies of the influence of Mo in pitting resistance of stainless steel led to the development of pitting resistance equivalence numbers (PREN) that rank the resistance of steels to pitting corrosion. An example formula  is:
𝑃𝑅𝐸𝑁 = 𝐶𝑟% + 3.3 𝑀𝑜% + 16𝑁% Equation 2-15
Although the influence of Mo in preventing pitting is clearly quantifiable, the exact mechanism that causes this improvement is under debate. Three major theories have emerged.
1. Mo enriches the surface of the alloy preventing initiation and passive film
The oxide has order at the nanostructure level  that can be interpreted to be significant in pitting initiation. Mo has been observed using time-of-flight SIMS to be enriched in the passive layer during polarisation of Fe-17Cr-14.5Ni-2.3Mo alloy, existing mostly as Mo(IV) before polarisation and becoming enriched up to 16% of cations in the Mo(VI) state after polarisation.
2. Mo reduces dissolution rate, preventing pits from becoming stable during the
The theory of enrichment of corroding surfaces with Mo is well established . Newman found that on scratched surfaces of ferritic Fe-18.6%Cr stainless steel the addition of 2.5 wt% Mo reduced the dissolution rate in the active region, but only had a small effect on the passivation potential if passivation was indeed possible . Newman  surmised enrichment mainly occurred at the kink/step sites due to the small surface coverage of Mo. The suggestion that the potential needed to generate a salt layer may be higher was also made. Using 1D pits, Newman  showed that the anodic dissolution rate of austenitic stainless steels was 5-10 times lower under active (i.e. salt-free) dissolution in alloys when 1.6wt% Mo was added.
3. Mo causes polymeric networks near the dissolving interface, interrupting
diffusion kinetics within the pit solution.
Kimura et al. observed spectra from corroding Mo in chloride solutions using X-ray absorption spectroscopy. From these results they suggested that they
resembled results similar to Na2MoO4, and suggested a complex matrix of
molybdate species could form in the solution near the corrosion interface, preventing ion diffusion and retarding corrosion rates when alloyed with stainless steel.
However Davenport et al. used synchrotron-based X-ray absorption
spectroscopy near the corroding interface of 316L stainless steel to identify Mo(III) species in solution, with no evidence of Mo(VI) polymolybdates.
2.5.Atmospheric Pitting Corrosion
Whilst corrosion often occurs in full immersion conditions, it is possible for situations to occur where small amounts of solution are present on metal surfaces.
These solutions can have trace amounts of salt in them, creating conductive
electrolytes that promote corrosion. The restricted volume of the electrolyte in these cases often results in highly concentrated solutions forming, causing localised corrosion. This is known as atmospheric pitting corrosion.
2.5.1. Salt deposition
Salt is often found on the surfaces of structures, particularly if they have been through any form of transit or period of storage outdoors . The majority of salt that acts as catalyst for atmospheric corrosion arrives on the surface of the metal in one of two ways:
1. As an aerosol, e.g. from ocean waves crashing or other such nebulising activity, which deposit on the metal surfaces as solid particles of salt.
2. By being in a splash zone, where dilute saline solutions (e.g. sea water) are splashed onto metal surfaces.
In both cases, maintaining an aggressive solution to allow corrosion to occur relies on the property of salts known as deliquescence
‘Deliquescence’ is the process that a hygroscopic salt undergoes of drawing in moisture from the atmosphere to keep equilibrium between the water activities of the solution and the surrounding atmosphere . When humid air is present in a system with salt, an equilibrium in water activities will be reached between these two phases . Salt will draw in moisture if the atmosphere’s relative humidity (RH)
is higher that the salts Deliquescence Humidity (DH), and will expel moisture if RH is below DH. Losing moisture is known as ‘effluorescence’.
Each salt species has a unique DH . The deliquescence humidity is sensitive to temperature as it is a thermodynamic process. A consequence of maintaining
equilibrium in water activities between the atmosphere and the solution is that small volumes of solution will have their concentration controlled by the humidity of the atmosphere. A solution that is in an atmosphere with an RH that is equal to its salt’s DH will be, by definition, saturated.
Tsutsumi et al. showed 304L stainless steel is vulnerable to atmospheric corrosion when exposed to humidities of less than 65% RH, which is equivalent to approx. 3 M MgCl2 . While “dry” conditions are generally considered to be resistant to corrosion, Schildelholz et al. [113, 115] have shown that corrosion can occur on Fe at humidities well below RH for NaCl, MgCl2 and artificial sea water salt crystals.
2.5.3. Evans Droplet Model
Corrosion of Fe was investigated by Evans by depositing droplets of NaCl with a phenolphthalein/potassium ferrocyanide addition as pH indicators [116, 117]. Evans showed that as corrosion propagated a distinct high-pH region occurred around the edge of the droplet and a low-pH region occurred towards the centre where the metal dissolution occurred (Figure 2-6). This preferential location of corrosion was
determined to be the consequence of “differential aeration”, i.e. a concentration gradient of oxygen in solution . This gradient drives oxygen reduction, the main cathodic reaction, to occur at the edges of the droplet where the easiest supply of oxygen is, leaving the centre prone to metal dissolution. Chen and Mansfeld 
showed using a Kelvin probe cathodic potentials around the edge of NaCl droplet on steel, supporting this model.
Figure 2-6 Schematic diagram showing reactions occurring in the Evans Droplet Model. The anodic and cathodic regions are spatially distinct, with cathode at the edge of the droplet. Differences in pH are caused by reactions stated.
This behaviour has also been observed in Zn alloys under droplets of salty water , with corrosion occurring towards the centre of the droplet, which has been modelled by controlling oxygen diffusion as the dominant reduction reaction . Aluminium dissolution under droplets does not appear to conform to the Evans droplet model as no preferential site is observed [122, 123] . However, when pure DI water was deposited on AA2011 trenching was observed around Cu-rich inclusions around the droplet edge, indicating an alkaline region and thus oxygen reduction, that was not observed near the centre .
Stainless steel has not been observed to follow the Evans model, with pitting occurring without noticeable trend when under droplets of MgCl2 [125, 126]. This has been attributed to the very stable passive layer present on stainless steels. Other
alloys, such as Fe and Zn , have much less stable passive layers so corrosion is able to migrate as conditions change, which was observed by Evans on Fe . Some investigations using wire beam electrodes have noted that in some conditions corrosion of both Fe and 304L stainless steel can occur towards the edge of droplets [128, 129] if droplets are sufficiently large at deposition.
2.5.4. Secondary spreading of droplets
A common occurrence in atmospheric corrosion under droplets is secondary spreading of droplets during corrosion. Secondary spreading is usually a solution layer on the order of monolayers thick and has been observed to participate in corrosion electrochemistry, increasing the cathodic area . The salt species used can heavily influence secondary spreading. NaCl has been shown to promote the secondary spreading of droplets [121, 130], while MgCl2 solutions did not spread. This was suggested to be due to insoluble Mg(OH)2 pinning the boundary of the droplet.
Micro-droplets have been observed to form around deposited droplets during corrosion , with external polarisation of droplets has been observed to increase the expansion of secondary spreading and the formation of “micro-droplets” . This result was confirmed on carbon steel and stainless steel using bi-plate
Micro-droplets have also been shown to appear above anodic attack, with “filiform-like” corrosion occurring under MgCl2 micro-droplets on 304L  and
hemispherical pitting on AA7075 . There is evidence that these micro-droplets are caused by anodic dissolution, as the ejection of metal ions into solution has been observed to cause droplets under thin films of solution .
30 2.5.5. Laboratory simulation
220.127.116.11. Laboratory salt deposition
Using droplets of dilute saline solutions is a common method of depositing of salt onto a sample surface, and deposition is usually by micropipette or syringe [114, 136]. Droplets are useful because geometries are often very well defined, making it easy to isolate influences on anodic and cathodic regions. It is also easy to calculate Chloride Deposition Density (CDD), which is the mass of chloride over area, usually written in units of μg/cm2 [2, 137]. CDD is an industry standard used to quantify the amount of salt found on structures, so using droplets allows direct comparisons to practical experience.
Using droplets also presents challenges. The deposition of dilute solutions does not necessarily reflect the “deliquescence” processes that occur in practice, where solid salt draws in moisture from the atmosphere and its liquid phase starts at saturation. Other techniques have been attempted to investigate this, such as inkjet printing of salt onto metal surfaces [138-140] or the direct deposition of fine salt particles [141, 142] . High pressure N2 gas has been used to atomise salt and deposit on metal surfaces through a cascade impactor , as has using ethanol as a medium to deposit salt has also been used [144, 145].
18.104.22.168. Electrochemical measurements of atmospheric corrosion
Electrochemical measurements of atmospheric corrosion are technically challenging due to the restricted volume of solution available. The Kelvin Probe (KP) is a non-contact technique pioneered by Stratmann et al.[146-148] initially used to investigate Fe and Fe-Cu systems. The vibrating probe is held above the sample and local
potentials can be measured, with anodic and cathodic sites along the surface able to be isolated spatially. Chen and Mansfeld  first used a KP to show cathodic regions on steel can extend to outside the droplet perimeter. Neufeld et al.  also showed this secondary spreading on Zn and monitored its spread over time noting an increasing participation in cathodic current. Tsuru et al.  used KP to show that micro-droplets that occur in the secondary spread region adjacent to droplets provide cathodic current with the main droplet being anodic.
Other techniques have also been used to investigate the onset of corrosion though they do not possess the ability to isolate anodic sites on the metal surface. Co-planar electrodes connected across a zero-resistance ammeter that allow the moment current begins to flow between the plates to be seen [132, 149, 150]. This has been extended to use 2D arrays of wire to construct wire-beam electrodes [128, 151] to try to collect data on different positions under droplets of solution.
Nam et al.  used a Ag-wire electrode across the surface of droplets of MgCl2 on 304 and 430 stainless steels to show the effect of humidity on initiation and
repassivation. By holding a Ag-wire across a droplet and connecting it and the sample plate to a two-electrode potentiostat, the range where pitting occurred was able to be isolated. On 304 it was shown to be 47-58% RH at 298K, and 48%-68% on 430. Repassivation occurred at higher RH, i.e. lower solution concentration, with 304 repassivating between 56%-70% RH and 430 between 67%-73% RH at 298K
2.5.6. Morphology of pits
The shape of pits in corrosion varies depending on the conditions they are generated under. Pits grown in full immersion conditions under applied potentials often require
occlusion to propagate. Schwenk  observed hemispherical pits in the initial stages of growth covered with a porous layer that acted as a diffusion barrier, though these pits sometimes showed faceting if initiated away from the edge of grain
boundaries. They then developed into hemispherical shapes and lost their faceted appearance . These porous layers, sometimes described as “lacy covers” , were also found in dilute chloride solutions described as Lacy pit covers on stainless steels [153-155] and Fe .
Pit morphology is influenced by microstructure, with orientation of inclusions and other phases, such as δ-ferrite bands, affecting propagation in stainless steels . Solution concentration has been seen to affect pit mouth size and modelling has confirmed the influence of solution concentration on repassivation kinetics [8, 158]. Applied potential can also influence pit morphology, with higher potentials often giving smoother pitting surfaces [17, 159]. Sato [160, 161] observed crystallographic etching in pitting of Fe when at low applied potential that smoothed out then
potential was increase, and attributed this to the development of a critical concentration inside the pit.
Pits that have grown in atmospheric conditions, and that have developed at OCP, have shown different morphologies than those grown under applied potential. Maier and Frankel  showed that pitting of 304L under droplets of MgCl2 often had shallow dish regions, developed by a process called “earing” due to the ear-shaped morphology observed in the early stages of attack. This observation was also
reported by Hastuty et al  on 430SS. The shallow dish regions are interesting in that they are broadly unoccluded. Cruz et al.  observed “colonies” of smaller pits around a large, flat region of attack. Mi et al.  saw that the size of these pits
grew with increasing droplet surface area, indicating a cathodically limited attack .
2.6.1. What is a synchrotron?
A synchrotron is an electron accelerator that is used as a very high quality X-ray source, providing both excellent flux and consistency compared to normal laboratory sources  (Figure 2-7).
Figure 2-7 Schematic diagram of a third-generation synchrotron .
Electrons are generated in a vacuum at an “electron gun” using a process known as “thermiomic emission” that applies an anodic voltage across a cathodic heater, propelling electrons in the synchrotron. Electrons are then fed into a Linear
Accelerator (LinAc) to an energy of ~100 MeV. The electrons then enter a booster ring where they are further accelerated before entering the storage ring.
The storage ring is not a “ring” but a polygon that uses bending magnets to deflect the electrons. The storage ring is designed to have a constant current, and is topped up from the boosting periodically as electrons are lost by use or hitting residual gas in the vacuum. Electrons are accessed by “insertion devices” that are used to generate X-rays.
Insertion devices have arrays of magnets lined up with opposite poles. As the electrons move passed these arrays of magnets, they begin to “wiggle” and give off energy in the form of X-radiation as they continually change direction. As the electrons are travelling at relativistic speeds, causes the radiation to be directed forwards, creating an X-ray beam of high flux, brightness (intensity per unit area of source) and spectral brightness (intensity per unit area per unit solid angle per unit energy bandwidth).
The beam that comes out of the insertion device is known as “pink beam” as it has a wide range of wavelengths. It is possible to refine and select the wavelength of the radiation in the “optics” hutch, before experimental use, by using a monochromator. Monochromators use two  or four  Si (111) crystals to select energy by serial diffraction. By aligning the crystal at specific angles, it is possible to select a single wavelength of radiation by using Bragg’s law .
2.6.2. X-ray Diffraction on corrosion systems
X-ray diffraction allows the identification of crystalline phases by their diffraction patterns. Crystalline structures are arranged in such a way that their atoms form sheets or layers with fixed spacing. When X-rays interact with these layers, they give
constructive interference and diffract in discrete patterns, which are determined by Bragg’s law:
𝑛𝑖𝜆 = 2𝑑𝑠𝑖𝑛𝜃 Equation 2-16
Where ni is any integer, λ is the radiation wavelength, d is the layer spacing, and θ is the angle of incidence.
Most salt layers are crystalline (some are molten), and synchrotron X-ray diffraction has been used to observe these salts in situ. Rayment et al.  has used artificial pits of Fe and 316L in 1 M HCl to show a FeCl2.4H2O salt exists during dissolution. Information was also able to be found about the morphology of the salt crystals in the pit, with 316L showing significantly more spottiness in the collected diffraction pattern indicating a coarsening of crystal size. Xu [6, 69] also use a similar technique to compare salt layers of Fe in NaCl with and without nitrate additions, finding that nitrate increases anisotropy of salt crystals. Other groups have investigated salt layers on copper  and scale in carbon steels .
X-ray Radiography can be used to view changes in morphology in situ. The X-ray beam can pass through a sample and be attenuated, i.e. lose flux due to absorption or deflection. The amount of flux lost due to attenuation is usually quantified in terms of a ratio of the original beam:
𝐼𝑛𝑡0 = exp (−𝜇𝑥𝑡) Equation 2-17
Where Int is the transmitted beam intensity, Int0 is the original beam intensity, μ is the absorption coefficient of the material and xt is the thickness of the material. The
transmitted beam hits a detector, either an undeveloped film or a fluorescent screen in more modern instances, and produces a two-dimensional image.
In its raw state, this image may not accurately represent the experiment as it contains distortions due to changes in the beam (flat field) and heterogeneities in the detector (dark field). Radiographs are typically corrected after collection by subtracting any contribution of the dark field and dividing through any contribution of the white field. The flat field is usually an average of several images of the x-ray beam without a sample present.
𝑐𝑜𝑟𝑟𝑒𝑐𝑡𝑒𝑑 𝑑𝑎𝑡𝑎 =𝑡𝑟𝑎𝑛𝑠𝑚𝑖𝑡𝑡𝑒𝑑 𝑑𝑎𝑡𝑎−𝑑𝑎𝑟𝑘 𝑓𝑖𝑒𝑙𝑑
𝑓𝑙𝑎𝑡 𝑓𝑖𝑒𝑙𝑑−𝑑𝑎𝑟𝑘 𝑓𝑖𝑒𝑙𝑑 Equation 2-18
Radiography has been used to investigate the growth of artificial pits in situ, with Ghahari et al.[8, 10, 171] investigating the dissolution kinetics of 304L to inform their kinetics model. Hammons et al.  has also used the technique on Ni to characterise consistency in the dissolution of the interface during corrosion.
2.6.4. Effect of X-radiation on electrochemical data
Xu  has previous addressed the paucity of work done on the influence of a high flux of radiation on corrosion processes. Nagy and You  have reported on the extent of radiolysis found in in situ synchrotron experiments involving solutions. Radiolysis will always occur, with the generation of H2 and H2O2 as a consequence. Particular concern is in cells with narrow geometries, as most radiolysed solution will stay at the working interface. The effect is broadly mitigated by attenuating the radiation beam by use of Al filters .
304L and 316L stainless steels were obtained from Goodfellow, Aperam, and Advent. Details are shown in Table 3-1.
Table 3-1 Alloys used in this body of work
Material Form Supplier Thickness Processing Composition (wt%)
Foil Goodfellow 25 μm and 50 μm Annealed Cr-18%, Ni 10%, C <300 ppm , Fe balance Synchrotron XRD and radiography Sheet Aperam 3 mm Cold-rolled,
solution annealed at 1040-1100 °C then air cooled Cr 18-19.5%, Ni 8-10.5%, Mn 2%, S 0.015% max N 0.1% Max, C 0.03% max, P 0.045% max, Fe balance Atmospheric droplets exp morphology and position, full immersion plate, Ag wire experiment
Wire Advent 50 μm Temper
annealed Cr 17-20%, Ni 8-11%, C<300 ppm, Fe balance 1D pitting
Wire Advent 125 μm Temper
Annealed Cr 17-20%, Ni 8-11%, C<300 ppm, Fe balance Wire experiments 316L
Wire Advent 50 μm Temper
annealed Cr 17-20%, Ni 8-11%, Mn 2% max, C<300 ppm, Fe Balance 1D pitting
Wire Advent 125 μm Temper
annealed Cr 17-20%, Ni 8-11%, Mn 2% max, C<300 ppm, Fe Balance Wire Experiments
38 3.1.1 SEM and EDS characterisation of alloys
Plate steel supplied for these droplet tests was electro-arc melted then continuous casted, cold-rolled and annealed. SEM analysis of 304L plate stainless steel is shown in Figure 3-1, where the plate has been mirror polished using OP-S (Struers) for 10 min, leaving a slightly etched surface. The plate is almost entirely populated with equiaxed grains, with a distribution of annealing twins throughout the surface. Sheet steel would be expected to have elongated grain structure as it goes through rolling processes after casting , but the foundry note supplied with this plate steel showed that it had been annealed after rolling at 1040 - 1100 °C, allowing
recrystallisation of the grains and producing an equiaxed grain structure of austenite.
Figure 3-1 Secondary electron Scanning Electron Microscope image of mirror polished 304L plate stainless steel on the longitudinal surface. Surface polished with OP-S 0.04 μm colloidal suspension (Struers) for 10 minutes. Metallography shows equiaxed grains with annealing twins throughout the microstructure. Surface-breaking inclusions (circled) can be observed as stringers elongated along the rolling direction.
Figure 3-2 Energy Dispersive X-ray Spectroscopy of a surface-breaking inclusion on 304L stainless steel plate. Inclusion shows enrichment of S and Mn.
Table 3-2 Foundry specifications of 304L plate used in atmospheric corrosion experiments and EDS of plate alloy used. EDS of 304L and 316l wires used in electrochemistry experiments also shown
Element (wt %) Fe Ni Cr Mn S C Si N P Mo
304L Plate -
Foundry spec. (max) Bal 10.5 8- 19.5 18- 2 0.015 0.03 0.75 0.1 0.045 - 304L Plate -
Foundry analysis Bal 8 18.1 1.46 0.0033 0.023 0.44 0.072 0.032 - 304L Plate - EDS (3
point scan avg)
Bal 7.5 18.8 1.6 - - 0.47 - - -
304L wire - EDS (3 point scan avg)
Bal 9.8 19.8 0.7 - - 0.46 - - -
316L wire - EDS
EDS analysis of these inclusions (Figure 3-2) showed that these were rich in Mn and S. The composition of the plate alloy can be seen in Table 3-2. Composition of 304L and 316L wires used in electrochemistry are also shown in Table 3-2.
NaCl + NaNO3 and MgCl2 solutions were used in these experiments. For
synchrotron experiments, 1 M NaCl + NaNO3 solutions were used, where NaNO3 concentration ranged between 0 and 75 mM. For atmospheric corrosion experiments using droplets, MgCl2 concentrations ranging from 0.03 M to 5 M were used. For full immersion experiments, MgCl2 solution concentrations ranging from 1 M to 5 M MgCl2 were used. All MgCl2 solutions were made using MgCl2.6H2O (Sigma
Aldrich or Fisher Scientific) and deionised water (Millipore, >15 MΩ cm). NaCl solutions were made using NaCl (Sigma Aldrich), NaNO3 (Sigma Aldrich) and deionised water (Millipore, >15 MΩ cm).
3.3.1. Synchrotron sample preparation
The same 2D foil samples were constructed for synchrotron XRD and radiography experiments, as described by Rayment et al.. Approx. 3 mm wide strips of 50 μm thick (for XRD) and 25 μm thick (for radiography) 304L stainless steel (Goodfellow) was cut and degreased in methanol for 15 minutes before air-drying. These foils were then embedded in Araldite epoxy resin (3M). Once dry, the foil was cut in two and the freshly cut surface became the pit mouth and was attached to a reservoir using Kapton tape (3M) (Figure 3-3).